Turning a "useless" ligand into a "useful" ligand

While the phenolic oximes (R-saoH 2 ) are well known for producing monometallic complexes of the type [M II (R-saoH) 2 ] with Cu II ions in near quantitative yield, their derivatisation opens the door to much more varied and interesting coordination chemistry. Here we show that combining the complimentary diethanolamine and phenolic oxime moieties into one organic framework (H 4 L 1 and H 4 L 2 ) allows for the preparation and isolation of an unusual family of [Cu II ] n wheels, including saddle-shaped, single-stranded [Cu II8 ] wheels of general formula [Cu 8 (HL 1 ) 4 (X) 4 ] n [Y] (when n = 0, X = Cl − , NO 3 − , AcO − , N 3 − ; when n = 2+ X = (OAc) 2 /(2,2’-bpy) 2 and Y = [BF 4 ] 2 ) and [Cu 8 (HL 2 ) 4 (X) 4 ] (X = Cl − , Br − ), a rectangular [Cu 6 (HL 1 ) 4 ] wheel, and a heterometallic [Cu 4 Na 2 (HL 1 ) 2 (H 2 L 1 ) 2 ] hexagon. Magnetic studies show very strong antiferromagnetic exchange between neighbouring metal ions, leading to diamagnetic ground states in all cases. DFT studies reveal that the magnitude of the exchange constants are correlated to the Cu-N-O-Cu dihedral angles, which in turn are correlated to the planarity/puckering of the [Cu II ] n rings.


Introduction
2][3][4][5] The ease of synthesis of new compounds permitted the facile preparation of families of related molecules, providing simple (s = 1/2) model systems with which to test emerging theories and propose new experiments. 1In 1952 Bleaney and Bowers published a study of the magnetic properties of copper(II) acetate monohydrate, 2 and some twenty three years later Hatfield and Hodgson published a magneto-structural correlation (MSC) demonstrating the linear relationship between the strength of the magnetic exchange interaction, J, and the Cu-O-Cu bridging angle in an extended family of bis(μ-hydroxido)copper(II) dimers. 3,4The first pre-designed construction of a molecule containing ferromagnetically coupled metal ions then followed in 1978 with the molecule [CuVO(fsa) 2 en] (where (fsa) 2 en 4− is the bi-chelating ligand derived from the Schiff-base bis-(2′-hydroxy-3′-carboxybenzylidene)-1,2-diaminoethane) in which the magnetic orbitals on the constituent metal ions were rigorously orthogonal. 5The modern era has seen researchers turning their attention to increasingly more complex systems to examine, for example, spin frustration effects in Archimedean and Platonic solids such as Cu II cuboctahedra, 6 and spin-electric coupling in antiferromagnetic [Cu II 3 ] triangles resulting from the interplay between exchange, spin-orbit coupling and spin chirality. 7n the sixty or so years since the initial magnetic study of [Cu(OAc) 2 •H 2 O] 2 numerous different ligand types have been employed to construct molecules containing multiple Cu II ions. 8However, one ligand type which can be almost entirely excluded from this list are the phenolic oximes (R-saoH 2 ), since they have been shown to have an overwhelming propensity to form mononuclear complexes of the type [Cu(R-saoH) 2 ] in near quantitative yields. 9Indeed their remarkable selectivity for copper in the 2+ oxidation state has been exploited in industrial hydrometallurgy, with almost a quarter of the world's copper production involving salicylaldoxime-based ligands. 9This peculiar selectivity can be ascribed to the tendency of the ligands to form hydrogen bonded head-to-tail dimers mediated via intermolecular interactions between the oximic hydrogen atom on one unit and the phenolic oxygen atom of its neighbour (Fig. 1).The resulting pseudo-macrocyclic cavity facilitates metal complexation, and selectivity for Cu II arises from the goodness-of-fit of this metal cation with the cavity. 10iven the above, it is perhaps unsurprising that a search of the CSD reveals that there is only one example of a polymetallic Cu II cage containing two or more metal ions stabilised solely by phenolic oximes. 11The complex, [Cu 6 (L3-2H) 3 (μ 3 -O)-(μ 3 -OH)](PF 6 ) 3 , describes two [Cu II 3 O] triangles linked by three "double-headed" phenolic oximes, and forms when the ligand : metal ratio employed in the reaction mixture is low; i.e. when the metal ions are present in excess. 11Perhaps the historical observation of a lack of variety in the coordination chemistry of Cu II with phenolic oximes has prevented others from investigating the chemistry further, but the formation of the hexametallic Cu II 6 species is clear evidence that more interesting structures remain undiscovered.Indeed the [Cu II 3 O-(oxime) 3 ] triangles of the hexametallic cage are entirely analogous to the building blocks previously observed for Mn III , Fe III and Cr III ; all of which present more varied and more interesting structural and physical chemistry. 12In order to address this "misperception" and to prove that polymetallic cages of Cu II can be built with this ligand type, we have adopted a synthetic approach which has already proven successful in Mn chemistry. 13While both salicylaldoxime and diethanolamine have very limited track records in Cu II chemistry (a CSD search for the latter also returns only monometallic complexes) their combination into one single organic structural framework has the potential to transform the coordination abilities of both.Herein we show that this complimentary ligand approach to constructing novel polymetallic cluster compounds works rather well, by presenting the synthesis, structures and magnetic behaviour of a large and unusual family of Cu II -based wheels constructed using the pro-ligands H 4 L 1 and H 4 L 2 (Fig. 2).

X-ray crystallography
Single crystal X-ray diffraction data of 1-9 were collected at 100 K on a Agilent Technologies SuperNova at temperatures between 200 and 120 K. See Table S1 † and CIF files for full details.CCDC 991823-991828 and CCDC 1029554-1029556.

Results and discussion
Complexes 1-7 (Fig. 3-5) share the same general structural framework, and so for the sake of brevity we describe 1 in detail and highlight any significant structural differences present in 2-7.
The metallic skeleton of complex 1 (Fig. 3) describes a saddle-like or basket shaped, single-stranded, octametallic wheel of approximate radius 7.  The introduction of an Et-group (H 4 L 2 ) as opposed to a Megroup (H 4 L 1 ) at the oximic carbon atom of the ligand appears to exert little structural effect, with complexes 6 and 7 being largely analogous to 1, with minor changes in bond lengths and bond angles.Complexes 1-7 all contain terminally bonded or chelating anions, introduced to the reaction mixture in the copper salt.In order to examine the effect of removing this anion, we repeated the synthesis employing the methoxide salt of Cu II .The reaction between anhydrous Cu (OMe)   A repetition of the reaction that produces complex 8, but using Cu(BF 4 ) 2 •3H 2 O in place of anhydrous Cu(OMe) 2 and employing NaOMe instead of NEt 3 results in the formation of [Cu 4 Na 2 (HL 1 ) 2 (H 2 L 1 ) 2 ] (9; Fig. 6).The metallic skeleton of complex 9 also describes a hexametallic wheel, but on this occasion it is heterometallic, more hexagonal than rectangular, and non-planar.The asymmetric unit includes the Cu 2 Na trimeric moiety, (Cu1-Na1, ∼6.4 Å; Cu1-Na1′, ∼3.2 Å) with the Na…Na diameter of the wheel being ∼6.9 Å, and the closest Cu…Cu distance ∼4.9 Å (Cu2…Cu2′).Cu1 is five coordinate and trigonal bipyramidal (τ = 0.14), whilst Cu2 is four-coordinate and square planar in geometry.The ligands are of two types: HL 1 3− and H 2 L 1 2− (Fig. 6E and 6F).The former bridges a total of four metal centres, with the oximic and phenolic moieties μ-bridging (Cu-N-O-Cu; ∼50°; Cu-O-Cu, ∼112°), one alkoxide arm of the diethylamine moiety is μ-bridging between Cu1 and Na1′, with the second arm terminally bonded to Cu1 and H-bonded to a neighbouring oximic O-atom (∼2.6 Å).The second ligand uses its oximic O-atom (O6) to bridge between Cu1 and Na1; its oximic N-atom also bonded to Cu1.The phenoxide O-atom μ-bridges between Cu2 and Na1, with both diethanolamine arms being terminally bonded to Na1.The Na + ions are six-coordinate and in distorted octahedral geometries.There are two intramolecular H-bonding interactions per molecule; between the H-atom of the protonated diol arm of one ligand and the oximic O-atom of its symmetry equivalent (O⋯H = ∼2.6Å°).The closest intercluster contacts are between the coordinated O-atom of one diethanolamine arm and the CH 2 groups of a neighbouring arm (∼3.2 Å; Fig. S4 and S5 in the ESI †).Complex 9 is clearly rather similar in structure to complex 8, the major difference being the introduction of the larger Na + ions in the former.This has the effect of severely twisting of the M-M-M trimer of the asymmetric unit, from ∠Cu-Cu-Cu = 166°for 8 to ∠Cu-Cu-Na = ∼146°in 9.This has two consequences for the latter complex: firstly the metallic skeleton becomes more bowl-shaped, and secondly there are no longer any coplanar ligands lying perpendicular to the M 6 mean plane.Indeed the para-Me(Ph) moieties now point outward rather than inward as seen in all the previous cages (compare Fig. 5B and 6B).
It is difficult at this stage to definitively correlate the changes in syntheses, as summarised in Fig. 7, to the observed structural changes.The simplest reaction is that between Cu(OMe) 2 and H 4 L 1 , which produces [Cu 6 (HL) 4 ] (8) and MeOH.The same product results from reactions employing different alkoxide precursors.Thus it seems the alcohol produced does not bond to the Cu II ions.When the anion of the metal salt is changed to one that is commonly found to chelate, bond terminally or even bridge between metal centres, or if that anion is added separately to the reaction mixture (halide, pseudohalide, carboxylate), the nuclearity of the cage increases to [Cu 8 ] despite the fact that this anion is non-bridging.Much of this seems rather counter-intuitive at first: one might expect the removal of terminally bonded anions to promote increased bridging of HL 1 3− and/or to encourage further deprotonation to L 1 4− .However this does not occur, and even the addition of an excess of base does not achieve this transformation.We can only surmise that the addition of a bonding anion forces a change in the metal geometry which in turn forces a change in the bonding mode of the ligand and thus to different cluster nuclearities and topologies.The introduction of the alkali metal ion Na + , in the form of NaOMe, suggests other heterometallic cages can be made by simply employing alternative group 1 or group 2 alkoxides, although we have not investigated this further.A search of the CSD reveals that there are thirteen examples of O-bridged, single-stranded homo-metallic Cu II wheels of nuclearity ≤ 8 in the literature.2][23][24][25][26] There are many more examples of both octametallic and hexametallic singlestranded Cu wheels which contain bridging motifs that do not feature oxygen atoms. 27To the best of our knowledge there are no reported examples of single-stranded heterometallic wheels of nuclearity six with a Cu : M (where M is an alkali metal cation) ratio of 4 : 2. Complexes 1-7 therefore become only the 12th examples of O-bridged single-stranded octametallic Cu II wheels, complex 8 only the 7th example of a single-stranded hexametallic Cu II wheel, and complex 9 the first example of a single-stranded heterometallic Na/Cu II wheel.Apart from their rather beautiful structural aesthetics, molecular wheels have long held fascination for both chemists and physicists, since they can often act as model compounds for the study of quantum effects and spin frustration. 28and have recently been identified as potential candidates for quantum information processing. 29gnetochemistry DC magnetic susceptibility.Dc magnetic susceptibility measurements were collected for complexes 1, 2, 8 and 9, in the T = 300-5 K temperature range in an applied field of B = 0.1 T. The data are plotted in Fig. 8 as the χ M T versus T products.1 and 2 are representative examples of the two structurally different Cu 8 wheels, with 8 and 9 being the Cu 6 and Cu 4 Na 2 wheels, respectively.The data for all four complexes are rather similarshowing a rapid decrease in χ M T with decreasing temperature, indicative of the presence of very strong antiferromagnetic interactions between neighbouring Cu II ions, resulting in diamagnetic ground states (at T = 110-220 K) in all cases.We have used the programme ITO-MAGFIT 30 which makes use of irreducible tensor operator algebra 31 to block-diagonalise the spin-Hamiltonian in order to model the experimental data.In all cases the g-values of the Cu(II) ions were fixed to g = 2.2.The resulting best-fit curves obtained in this way are shown as solid black lines in Fig. 8 with the corresponding best-fit parameters listed in Table 1.A schematic of the models employed is shown in Fig. 9.For the Cu 8 clusters best-fit J-values reveal that the exchange through the Cu-O/NO-Cu bridge is very large and negative ( J 1 = −457 and −302 cm −1 for 1 and 2 respectively), with the exchange through the Cu-O-Cu bridge also antiferromagnetic but smaller in magnitude ( J 2 = −20.1 and −38.9 cm −1 for 1 and 2 respectively).The differences can be correlated to subtle differ-Fig.7 Summarising the effect changes in CuX 2 starting material has on product formation with H 4 L 1/2 .Fig. 8 The magnetic susceptibility data, as χ M T, versus T at B = 0.1 T for complexes 1 (red), 2 (green), 8 (blue) and 9 (magenta).The solid black lines are fits of the experimental data.The best fit 3J model is shown for 8. See text for details.
Table 1 Comparison of J values obtained from the fitting of experimental data to the models depicted in Fig. 9, and those from DFT calculations ).The former would be expected to make J 2 larger in 1, and the latter make J 1 larger in 2, as observed.For complex 8, the best fit of the experimental data is afforded by a 3J model, accounting for the single alkoxide bridge ( J 1 ) and the two NO/O bridges which display markedly different bridging angles (48.17, 37.47; J 2 and J 3 ).The best fit parameters obtained were J 1 = −107, J 2 = −239 and J 3 = −260 cm −1 .This fit however is not unique and we were able to obtain several satisfactory fits using a 2J model (see Table 1).Nevertheless, the parameters of the 3J best fit are consistent with those obtained for 1 and 2 in which J (O/NO) > J (O) and with the larger torsion angle mediating weaker antiferromagnetic exchange.Complex 9 describes a wheel comprising two simple, non-interacting Cu(II) dimers in which we assume negligible interaction through the Cu-Na-Cu bridge.This model affords a best fit J 2 = −271 cm −1 .The exchange is again antiferromagnetic in nature, but somewhat larger than observed for 1, 2 and 8.A literature search reveals only three examples of dimers which feature Cu-O/NO-Cu moieties, but on which no magnetic studies have been reported. 32There are several examples of polymetallic Cu systems featuring Cu-O/NO-Cu bridging motifs, 33 and all show the interaction to be strongly antiferromagnetic.The magnitude of the exchange interaction in purely alkoxo-bridged Cu(II) dimers varies enormously and is dependent on the Cu-O-Cu angle, but in general they tend to be strongly antiferromagnetic with J lying in the region −200 to −1000 cm −1 . 34A similar pattern is seen in purely oximato bridged Cu(II) dimers, where J ranges from −361 cm −1 to −880 cm −1 , 35 although in the vast majority of cases J appears to lie in the region −600 to −800 cm −1 .In order to investigate the origin and magnitude of the exchange interactions seen in complexes 1, 2, 8 and 9 further we have turned to theory, and now discuss a computational DFT study.
Theoretical studies Computational details.Calculations were performed using the B3LYP 36 functional, with Alhrich's triple-ζ TZV 37 basis set for the Cu(II) ions and SV basis sets for the remaining atoms, as implemented in the Gaussian 09 38 suite of programs.0][41][42] The exchange Hamiltonians adopted are the same as those described in the experimental section above (Fig. 9).In complex 1 there are two unique exchange interactions denoted as J 1 and J 2 , mediated via a μ-phenoxo bridge and a μ-alkoxo/ oxime bridge, respectively.Calculations yield J 1 = −45.0cm −1 and J 2 = −320 cm −1 .Both interactions are computed to be antiferromagnetic in nature with J 2 being very strong.To cross check, calculations were also performed using a diamagnetic substitution method whereby all metal centres not involved in the exchange interaction were replaced with diamagnetic Zn(II) ions.This method yielded a very similar set of J values, J 1 = −35.1 cm −1 and J 2 = −300 cm −1 .Fitting of the experimental susceptibility data also yields similar J values, indicating weak antiferromagnetic J 1 and strong antiferromagnetic J 2 interactions (see Table 1), as would be expected since their Cu-O-Cu angles are rather similar (115.8°,118.6°).However their magnitude is much smaller than might be anticipated from previous magnetostructural correlations. 43This results from the puckering of the ring: the unpaired electron in Cu(II) is found in the d x 2 −y 2 orbital and the buckled nature of the wheel results in the two magnetic orbitals (corresponding to the J 1 interaction) being in different planes (Fig. S6 †), weakening the interaction.This is in stark contrast to the J 2 interactions where the oxime moiety forces the d x 2 −y 2 orbitals to be in same plane, leading to a very strong interaction.The magnitude of exchange in Cu(II) complexes can be correlated directly to the energy gap between the symmetric and antisymmetric combinations of the d x 2 −y 2 orbitals.The oxime bridge present in J 2 produces a complementarity effect whereby the π* orbitals of the oxime interacts with the antisymmetric combination (Fig. 10), leading to a larger energy gap and hence to stronger antiferromagnetic coupling.
The overlap integrals, computed as 0.08 and 0.20 for J 1 and J 2 , respectively, confirm this.Computed spin density plots for complexes 1, 8, and 9 are shown in Fig. 11.The Cu(II) centres in complex 1 possess spin densities of 0.63 [Cu(1)] and 0.59 [Cu(2)], values substantially lower than the expected value of 1.0, revealing significant delocalisation (and hence strong exchange) of the unpaired spin onto the bridging ligands.The spin density on the bridging groups are also significant, 0.12 on the O-atom of the µ-alkoxide ( J 1 ), and 0.16 on the O-atom of the µ-alkoxide, and 0.13 and 0.10 for O and N atoms of the oxime bridge in the J 2 interaction.
For complex 2 calculations yield a similar set of exchange constants, although the J 2 interaction is computed to be slightly smaller (Table 1).The decrease in the magnitude of the J 2 interaction compared to complex 1 is found to correlate to the Cu-O-N-Cu dihedral angle.In complex 2 the bulkier, chelating nitrate groups cause a twist in the Cu-N-O-Cu dihedral leading to weaker d x 2 −y 2 − d x 2 −y 2 overlap and a reduction in the J values.The spin density on the Cu(II) centres in complex 2 are plotted in Fig. S7.† For complex 8 calculations yield J 1 = +5.53cm −1 , J 2 = −25.9cm −1 and J 3 = −120 cm −1 .The J 1 interaction is computed to be weakly ferromagnetic in nature, in contrast to that fitted experimentally.Here the Cu-O-Cu angle is relatively small (102.2°) and along with the large out-of-plane shift of the O-C(alkyl) group from the Cu-O-Cu-O plane (∼40.0°) the geometry is approaching that theoretically predicted to mediate ferromagnetic exchange; 44 the crossover area likely being the source of error in the theoretical calculation.J 2 and J 3 are antiferromagnetic in nature with J 3 being approximately five times larger.This is again correlated to the difference in the Cu-N-O-Cu dihedral angle, with smaller angles yielding stronger antiferromagnetic coupling.The magnitude of the J 2 and J 3 interactions are much smaller than that computed for complexes 1 and 2 due to the smaller ring sizethe Cu-N-O-Cu moieties being far more twisted than that found in complexes 1 and 2. For complex 9 the computed exchange constants are J 2 = −95.8cm −1 and J 4 = +0.08 cm −1 .The former is consistent with that observed in previous complexes, and the latter as expected for an interaction mediated through a diamagnetic Na + ion.Computed overlap integrals (0.26 and 0.005 for J 2 and J 4 , respectively) are consistent with this picture (Fig. S8 †).In all four complexes the strongest antiferromagnetic coupling constant is underestimated by DFT, the differences being particularly obvious when the other J values are small in magnitude.The underestimation of the exchange interactions in Cu(II) complexes by DFT has been highlighted previously, 45

Conclusions
The simple reaction of Cu(II) salts with diethanolamine-functionalised phenolic oximes has resulted in seven new examples of single-stranded octametallic Cu(II) wheels, one new example of a single-stranded hexametallic Cu(II) wheel, and the first reported example of a single-stranded hexametallic mixedmetal Na 2 Cu 4 wheel.The construction of polymetallic cages from ligand moieties normally associated with producing monometallic Cu(II) compounds is clear evidence that combining complimentary ligand types into one organic framework is a sensible methodology for building polymetallic cluster compounds.In each case the interaction between neighbouring metal ions was shown to be strongly antiferromagnetic.DFT calculations suggest the origin to be a complementarity effect due to the presence of the oxime bridge, in which smaller Cu-N-O-Cu dihedral angles yield larger exchange constants, which are inherently linked to the planarity of the wheel.A magnetostructural correlation developed even suggests that such Cu(II) wheels can be made to display intramolecular ferromagnetic exchange if the Cu-N-O-Cu torsion angles can be of the order of 60°or larger.Current efforts are aimed at synthetic strategies to achieve just that.

Fig. 3
Fig. 3 The molecular structure of complex 1 viewed perpendicular (A) and parallel (B) to the Cu 8 "plane".Colour code, Cu = orange, O = red, N = blue, C = gold, Cl = green.(C) The metallic skeleton of 1 highlighting the bowl-shape of the cluster.(D) The magnetic core of 1 showing the two different exchange interactions.(E) The bridging mode of the HL 1 3− 2 and H 4 L 1 in a basic MeOH-MeCN solution afforded the homoleptic, hexametallic wheel [Cu 6 (HL 1 ) 4 ] (8; Fig. 5).The metallic skeleton of 8 describes a single-stranded hexametallic, rectangular Cu II wheel.The asymmetric unit contains half the wheel, i.e. three Cu ions (Cu1-3) and two HL 1 3− ligands.The latter are triply deprotonated as before, but coordinate differently in 8 than in 1-7.One ligand bridges a total of four and the other a total of three metal centres with the oximic and phenolic moieties μ-bridging (Cu-N-O-Cu, ∼37°, ∼48°; Cu-O-Cu; ∼108°, ∼113°) in both cases, as in 1-7.It is the alkoxide arms of the diethanolamine moiety of the two symmetry inequivalent ligands which behave differently: in one ligand, one arm is μ-bridging (Cu-O-Cu, 102.5°) with the other terminally bonded at the apical site of the Cu square-based pyramid (Cu-O, 2.35 Å); in the second, one arm is terminally bonded (Cu-O,

2. 4 Å
) and one non-bonded, and H-bonding to the bridging alkoxide from a neighbouring HL 3− ligand (O⋯O, ∼2.6 Å).The coordination geometries of the Cu ions are thus mixed: Cu2 is four coordinate and square planar, whilst Cu1 and Cu3 are five coordinate and square-based pyramidal (τ = 0.118 and 0.0775 respectively).The metallic skeleton is near planar, as opposed to the puckered structures of 1-7, with the short and long edges of the rectangle measuring ∼3 Å and ∼6 Å, respectively.As before, one pair of HL 1 3− ligands points above and one pair below the plane of the wheel, with the aromatic rings being separated by approximately 3.5 Å.The closest intermolecular interactions occur between the para-Me(Ph) groups of the ligand on one molecule and the terminally bonded O atom of the diethanolamine arms on its neighbour (∼3.7 Å, Fig. S3 †).

Fig. 6
Fig. 6 The molecular structure of complex 9 viewed perpendicular (A) and parallel (B) to the Cu 4 Na 2 "plane".Colour code, Cu = orange, Na = purple, O = red, N = blue, C = gold.(C) The metallic skeleton of 9 highlighting the bowl-shape of the cluster.(D) The magnetic core of 9 showing the two different exchange interactions.(E) The bridging mode of the H 1 L 3− ligand (F) The bridging mode of the H 1 L 3− ligand.H atoms omitted for clarity.

Fig. 9
Fig. 9 The magnetic cores of the representative Cu 8 , Cu 6 and Cu 4 Na 2 metal cores (left) and the models representing the exchange component of the spin-Hamiltonians which their experimental susceptibility data were fitted to (right).For the experimental fit of 9 J 4 = 0.
and is thus a limiting factor in the accurate estimation of absolute values.Since the Cu-N-O-Cu dihedral has been found to play an important role in determining the J values in this family of complexes, we have developed a magneto-structural correlation based on a dimeric model of complex 9 shown in the inset of Fig.12.By varying the Cu-N-O-Cu dihedral angle (x) [with the Cu-O-Cu angle fixed] from 0-80°an exponential correlation was found, with the smallest dihedral angles leading to the strongest AF exchange, and the largest dihedral angles leading to the weakest AF exchange.Fitting the data to the expressionÀ J ¼ Ae x t h i þ y oyields y o = −608, A = 262, t = −79.5,revealing a switch from AF to F exchange at dihedral angles >60°.Attempts are underway to isolate wheels with this large degree of puckering in order to test this theory.

Fig. 10
Fig. 10 Schematic representation of the complementarity effect exhibited by the oxime bridge with symmetric and antisymmetric combinations of d x 2 −y 2 orbitals (left) and a representative MO diagram depicting the antisymmetric combination of the d x 2 −y 2 orbitals (right).

Fig. 12
Fig. 12 Magnetostructural correlation developed by DFT calculations by varying the Cu-N-O-Cu dihedral angle in a model complex based on complex 9.The solid black squares are computed points and the red line the best fit to these points.The hollow blue circles are the DFT calculated values for the full structure, whilst the red circles are the experimentally fitted exchange constants.